Comparison of Effect of C-Factor on Bond Strength to Human Dentin Using Different Composite Resin Materials
Thakur Veerandar singh1, Jaya Prakash Patil2, RVS Chakradhar Raju3, Bhuvan Shome Venigalla4, SV Jyotsna5, Bhutani Neha6
ABSTRACT Background: The study was planned to assess the use of low shrinkage composites for restoring cavities with high configuration factor (C-factor) which are subjected to high stresses. Aim: The aim of the study was to evaluate the effect of C- factor on tensile bond strength to human dentin using methacrylate based nanohybrid and low shrinkage silorane composite. Materials and Methods: In this study 40 non carious human molar teeth were selected and assigned into two main groups - cavity (Class I cavity with high C-factor) and flat group (flat surface with low C-factor). Two different composite materialsmethacrylate based and silorane low shrinkage composite were used to restore the teeth. Dentin surface was treated, adhesive
application was done and composite was applied as per manufacturer’s instructions. Samples were stored in distilled water then subjected to tensile bond strength measurement using universal testing machine. Results: Statistical analysis was done using Independent sample t-test. The mean bond strength in methacrylate based and silorane composite was significantly higher in flat preparation (Low C-factor) than cavity preparation. The mean bond strength in both cavity (High C-factor) and flat preparation(Low C-factor) was significantly higher in silorane than in conventional methacrylate based composite. Conclusion: The bond strength of composites to dentin is strongly influenced by C-factor and type of composite resin material used.
Keywords: Bonding, Configuration factor, Polymerization, Shrinkage stress, Silorane composite, Tensilebond strength
Introduction Composites are most popular aesthetic restorative material used in dentistry but the major drawback is polymerization shrinkage which leads to undesirable clinical effects. C-factor is an important clinical consideration with regard to polymerization shrinkage, as it has implications on bond strength and bond integrity [1,2]. Studies have shown that with increase in C-factor the bond strength decreases [3,4]. Since there are few studies published in literature evaluating the effect of C-factor on bond strength of low shrinkage composite like silorane, the present study aimed at comparing the effect of C-factor on bond strength of methacrylate based and low shrinkage composite to human dentin.
Materials and Methods The present study was conducted in Department of Conservative Dentistry and Endodontics at Sri Sai College of dental surgery, Vikarabad in 2013. A total of 40 intact, non carious human molars which were extracted for periodontal reasons were selected for the study. They were subsequently debrided and examined to ensure that they were free of defects. They were stored in saline and used within 2 months. The occlusal surfaces of these teeth were ground using a diamond disc until all the occlusal enamel was removed. The prepared teeth were embedded into self-cure acrylic resin such that crowns were exposed. The teeth were randomly assigned into two main groups: cavity group and flat group. The cavity group represented a high C-factor group with Class I cavities and flat surface group represented a low C-factor group with flattened dentin surfaces. For high C-factor groups, Standardized class I occlusal cavity prearations (length: 4mm; width 4 mm; depth 2.5 mm) were made in each tooth with diamond burs using high speed contra angled hand piece. For low C-factor groups, flat dentin surface was exposed.
In each group samples were again sub divided into 2 groups. Two different types of composite resin materials were used in the study, Tetric N-Ceram representing methacrylate based composite and Filteksilorane representing low shrinkage composite. A total of 4 groups with 10 samples each were formed depending on type of cavity configuration and type of composite used. Group A– Cavity group restored with methacrylate based composite (Tetric N-Ceram). Group B – Flat group restored with methacrylate based composite (Tetric N-Ceram). Group C – Cavity group restored with low shrinkage composite (Filtek Silorane). Group D – Flat group restored with low shrinkage composite (FiltekSilorane). In Group A and Group C – The adhesive application was done in the respective groups as per the manufacturer’s instructions.A ligature wire of 26 gauge was taken and one end was twisted and at other end loop was formed. The twisted end was inserted inside the uncured resin. The composite resin was then light cured using LED light curing unit according to the manufacturer’s instructions. Following complete curing the adjacent tooth structure which formed the cavity walls was carefully removed using diamond burs under profuse water cooling, finally leaving a resin block with twisted wire bonded to the dentin surface. In Group B and Group D- A hollow polyvinyl mould having dimensions similar to that of class I cavity was held on adhesive treated flat surface of specimen and respective composite resin for each group was placed inside the customized mould and condensed. A ligature wire of 26 gauge was taken and one end was twisted and at other end loop was formed. The twisted end was inserted inside the uncured resin. The composite resin was then light cured using a LED light curing unit as per the manufacturer instructions. Journal of Clinical and Diagnostic Research. 2015 Aug, Vol-9(8): ZC88-ZC91
[Table/Fig-1]: Flat Dentin surface exposed [Table/Fig-2]: Adhesive application
Thakur Veerandar singh et al., Effect of C-factor on Bond Strength
[Table/Fig-3]: Composite packing in mould
[Table/Fig-4]: Light curing
Results The mean tensile bond strength in methacrylate based (Tetric N Ceram) and Silorane (Filteksilorane) composite was significantly higher in flat surface preparation (Low C-factor) than cavity preparation (High C-factor). The mean tensile bond strength in both cavity (High C-factor) and flat preparation (Low C-factor) was significantly higher in silorane (Filteksilorane) than in methacrylate based composite (Tetric N Ceram) [Table/Fig-7,8]. Preparation
[Table/Fig-5]: Prepared samples Composite
Tetric n ceram (methacrylate based)
Silorane (low shrinkage)
[Table/Fig-7]: Independent sample t-test for different types of composites Composite
Tetric n ceram (methacrylate based)
Silorane (low shrinkage)